**HAL Id: hal-01402004**

**https://hal.archives-ouvertes.fr/hal-01402004**

### Submitted on 28 Nov 2016

**HAL is a multi-disciplinary open access**

### archive for the deposit and dissemination of

### sci-entific research documents, whether they are

### pub-lished or not. The documents may come from

### teaching and research institutions in France or

### abroad, or from public or private research centers.

**L’archive ouverte pluridisciplinaire HAL, est**

### destinée au dépôt et à la diffusion de documents

### scientifiques de niveau recherche, publiés ou non,

### émanant des établissements d’enseignement et de

### recherche français ou étrangers, des laboratoires

### publics ou privés.

### Copyright

**Light-hole Exciton in Nanowire Quantum Dot**

### Mathieu Jeannin, Alberto Artioli, Pamela Rueda-Fonseca, Edith

### Bellet-Amalric, Kuntheak Kheng, Régis André, Serge Tatarenko, Joël Cibert,

### David Ferrand, Gilles Nogues

**To cite this version:**

### Mathieu Jeannin, Alberto Artioli, Pamela Rueda-Fonseca, Edith Bellet-Amalric, Kuntheak Kheng, et

### al.. Light-hole Exciton in Nanowire Quantum Dot. Physical Review B, American Physical Society,

### 2017, 95 (3), pp.035305. �10.1103/PhysRevB.95.035305�. �hal-01402004�

### Light-hole Exciton in Nanowire Quantum Dot

1

Mathieu Jeannin,1, 2 _{Alberto Artioli,}1, 2 _{Pamela Rueda-Fonseca,}1, 2, 3 _{Edith Bellet-Amalric,}1, 3 _{Kuntheak}

2

Kheng,1, 3 _{Régis André,}1, 2 _{Serge Tatarenko,}1, 2 _{Joël Cibert,}1, 2 _{David Ferrand,}1, 2 _{and Gilles Nogues}1, 2

3

1_{Univ.} _{Grenoble Alpes, F-38000 Grenoble, France}

4

2

CNRS, Inst. NEEL, "Nanophysique et semiconducteurs" group, F-38000 Grenoble, France

5

3

CEA, INAC, "Nanophysique et semiconducteurs" group, F-38000 Grenoble, France

6

Quantum dots inserted inside semiconductor nanowires are extremely promising candidates as building blocks for solid-state based quantum computation and communication. They provide very high crystalline and optical properties and offer a convenient geometry for electrical contacting. Having a complete determination and full control of their emission properties is one of the key goals of nanoscience researchers. Here we use strain as a tool to create in a single magnetic nanowire quantum dot a light-hole exciton, an optically active quasiparticle formed from a single electron bound to a single light hole. In this frame, we provide a general description of the mixing within the hole quadruplet induced by strain or confinement. A multi-instrumental combination of cathodo-luminescence, polarisation-resolved Fourier imaging and magneto-optical spectroscopy, allow us to fully characterize the hole ground state, including its valence band mixing with heavy hole states.

I. INTRODUCTION

7

Semiconductor quantum dots are seen as

impor-8

tant elements for integrated quantum simulation and

9

communication.1–3 _{They can act as static qubits, }

encod-10

ing information either onto their orbital or spin state.

11

They can also serve as a deterministic source of flying

12

qubits using single4,5 _{or entangled photons.}6–8 _{In this}

13

perspective, hole spins are particularly interesting

be-14

cause of their weak hyperfine coupling to surrounding

15

spin bath compared to electrons.9,10 _{Furthermore }

work-16

ing with light-holes pave the way to new information

17

technology protocols like direct manipulation of the hole

18

spin state with RF fields,11 _{efficient control of a }

mag-19

netic impurity spin coupled to a quantum dot,12 _{or spin}

20

state tomography of the electron inside the dot.13 _{}

How-21

ever most of the previous studies have concerned so far

22

heavy-hole states, because they are energetically favored

23

for a majority of quantum dot heterostructures for which

24

confinement and strain lift the degeneracy of the valence

25

band.14,15 _{Hence a way to address light-holes is to }

pro-26

mote them as the valence band ground state by

engineer-27

ing the strain inside the dot. For epitaxially grown dots

28

this requires technologically intensive methods, such as

29

the fabrication of deformable membranes containing the

30

dots.16_{Another very promising strategy is to embed the}

31

dot inside a nanowire.17 _{This bottom-up approach }

pro-32

duces high quality heterostructures. It offers a way to

33

control both the carriers confinement through the

ge-34

ometrical shape of the dot, and its internal strain by

35

adding a shell of a different material around the nanowire

36

core.18,19_{To be short, in most nanostructures the low-gap}

37

material has a larger lattice parameter. In a flat

quan-38

tum dot as resulting from Stranski-Krastanow growth,

39

it is well known that the hole ground state has a main

40

heavy-hole character. The most frequent case is that of

41

InAs dots in GaAs, but this is true also for CdTe dots in

42

ZnTe.20_{This is due to the stronger effect of confinement}

43

along the growth axis, and to the strongest component

44

of the mismatch strain which is compressive in the plane.

45

In a core-shell nanowire made of the same materials, the

46

confinement is stronger in the plane, and the strongest

47

component of the mismatch strain is compressive along

48

the axis. As a result, both confinement and mismatch

49

strain conspire to make the ground state a light-hole

50

state.19 _{When increasing the height of a quantum dot}

51

in a nanowire, a crossing is expected, from the

heavy-52

hole ground state in a flat quantum dot to a light-hole

53

ground state in an elongated quantum dot.18 _{Note that}

54

nanowire structures are very flexible, and a heavy-hole

55

ground state can be found also in a core-shell nanowire if

56

the lattice mismatch induces a tensile strain in the core.19

57

An additional important property of a semiconductor

58

nanowire is that it acts as a dielectric antenna,

modu-59

lating the coupling of the different exciton transitions to

60

light modes which changes their radiation pattern.5,21–24

61

Here we provide a complete study of a light-hole

quan-62

tum dot (QD) in a core-shell nanowire. The dot

con-63

tains a large fraction of magnetic dopants in order to

en-64

hance the Zeeman shift for spintronics applications. This

65

prevents a direct spectroscopic evidence of its light-hole

66

character by measuring its fine structure.16_{We show }

nev-67

ertheless that the detailed observation of the polarisation

68

state of the QD far field radiation pattern is enough to

69

prove its light-hole nature and provides a wealth of

in-70

formation about its mixing with heavy-hole states. Our

71

results are in agreement with numerical simulations of

72

the QD emission within the full nanowire structure. It

73

is confirmed by studying the giant Zeeman shift and the

74

polarisation of the excitonic transition under an external

75

magnetic field. The magneto-optical spectroscopy reveals

76

a heavy-hole excited state at high field, thus providing an

77

order of magnitude for the valence band splitting. Our

78

method is simple, and requires no extra processing of the

79

sample16,25 _{as far as the nanowire is isolated from its}

80

neighbours.

II. LIGHT-HOLE AND HEAVY-HOLE

82

PROPERTIES AND ANISOTROPY

83

Figure 1. (a), Energy levels inside the QD participating to the luminescence, along with the corresponding transitions with their oscillator strength and polarisation. (b), Schematic of the experiment. The light emission is mapped onto the Fourier plane to allow polarisation analysis of the photons with respect to the direction (θ, ϕ). The inset present a zoom of the nanowire in the vicinity of the quantum dot. (c,d), Theoretical far field intensity maps for the σ or π transition, respectively. The QD is assumed to be in an infinite space made of ZnTe. The green lines in (c) and (d) represent the time evolution the electric field in the (x, y) plane for a set of directions. For each direction the electric field origin is centered on the (θ, ϕ) coordinate.

The distinction between light- and heavy-hole arises

84

when the top of the valence band fourfold degeneracy

85

of zinc-blende semiconductors is lifted by, for instance,

86

strain or confinement. Generally, a relevant axis of

87

symmetry z appears, such as the growth axis for

self-88

assembled quantum dots or a nanowire. Eigenstates are

89

then Kramers doublets, characterized by the projection

90

of their total spin onto z for the electron (±1/2), the

91

light-hole (LH, ±1/2) and the heavy-hole (HH, ±3/2).

92

The HH has a strong magnetic anisotropy, with its spin

93

±3/2along z but a vanishing Landé factor in the normal

94

xy-plane. It exhibits also a strong optical anisotropy,

95

with dipolar electric transitions matrix elements towards

96

electron states in the xy-plane (called σ transitions

here-97

after), see Fig. 1(a). By contrast, the LH has a finite

98

Landé factor in the xy-plane and a smaller one along z.

99

Optically, it presents both σ and π polarised transition

100

matrix elements.

101

We use the hole formalism to describe the top of the

102

valence band: this is more convenient if one has in mind

103

the optical manipulation of holes in a quantum dot16 _{or}

104

carrier induced magnetic interactions in a dilute

mag-105

netic semiconductor.26_{As a result, the hole ground state}

106

is at lower energy, and the light-hole/heavy-hole

split-107

ting ∆LH is negative if the ground state is a light hole.

108

∆LH < 0 implies a LH ground state. However, in real

109

life quantum dot, confinement potential and strain

(uni-110

form and inhomogeneous) create additional anisotropy

111

components which break the circular symmetry around

112

z and hence mix the light- and heavy-hole states. This

113

mixing is usually described by two additional complex

114

numbers σe−iχ _{and ρe}−2iψ_{.}27 _{In appendix B, we show}

115

in details that the resulting 4 × 4 Hamiltonian, with one

116

real number ∆LH and two complex numbers ρe−2iψ and

117

σe−iχ, is the most general spin Hamiltonian describing

118

an isolated spin quadruplet and respecting time reversal

119

symmetry. All three terms have various origins, including

120

uniform and inhomogeneous strain, and confinement. As

121

a consequence of the mixing the true QD hole eigenstates

122

are linear combinations of the pure heavy- and light-hole

123

states defined by z, and the resulting dipole transitions

124

and spin properties are changed accordingly.

125

The spin Hamiltonian takes a much simpler form in

126

the frame (x0, y0, z0) which diagonalizes the anisotropy

127

tensor (see appendix B). It then depends only on two real

128

parameters: ∆LH0 which describes the LH/HH splitting

129

along the principal anisotropy axis z0 and ρ0 which

de-130

scribes the transverse anisotropy in the (x0, y0) plane.

131

Three Euler angles ˆα, ˆβ and ˆγ are necessary to

charac-132

terize the transformation from the laboratory frame to

133

the anisotropy frame. If ˆβ 1, ˆβ and ˆγ are the

spheri-134

cal coordinates (θ, ϕ) of axis z0. ˆα + ˆγ characterizes the

135

direction of transverse anisotropy. The parameter σ

mea-136

sured in the laboratory axes does not really represent a

137

mixing, but the result of the tilt ˆβ between z and z0.

138

We stress this physical interpretation of the two "mixing

139

parameters" measured in the laboratory frame, because

140

it has direct practical consequences: ρe−2iψ _{describes a}

141

real mixing, which requires that a shear strain be applied

142

in order to compensate for it.16 _{On the other hand the}

143

effect of σ (which can also be due to strain and

confine-144

ment anisotropy) can be compensated by an appropriate

145

tilt of the optical axis.

146

In our setup we collect the nanowire light by placing a

147

microscope objective (numerical aperture NA=0.72) on

148

the z axis [Fig. 1(b)]. A set of additional optical elements

149

allows to image onto a CCD camera the intensity I(θ, ϕ)

150

emitted in a direction (θ, ϕ).23,24_{Figures 1(c-d) represent}

151

the theoretical colormaps of I(θ, ϕ) for a σ and π

transi-152

tion respectively, assuming that the QD is surrounded by

153

an infinite medium made of ZnTe for illustration purpose

154

first. The radial coordinate is equal to sin θ and the polar

155

angle is equal to ϕ. The two radiation patterns differ

dra-156

matically, and could be enough to discriminate light- and

157

heavy-hole emission. Nevertheless, they are significantly

158

affected by the nanowire geometry and by the

imperfec-159

tion of the collection objective. Note that while the π

160

dipole emission does not radiate along the optical axis,

161

it does generate light towards larger angles within our

3

experimental numerical aperture, which is collected by

163

our objective [see Fig. 1(d)]. A more precise description

164

of the radiated field comes from the polarisation of the

165

light emitted in a given direction. It is projected by the

166

objective onto a state of polarisation in the (x, y) plane,

167

represented in Fig. 1(c-d) by the green curves which

fol-168

low the electric field vector E(θ, ϕ, t) over one optical

pe-169

riod. It results in an ellipse whose aspect ratio changes

170

from a perfect circle for a pure σ± _{to a single line for a}

171

pure linear polarisation state. Here again, striking

differ-172

ences exist between π and σ transitions. One important

173

message of our work is that this polarisation analysis for

174

a large set of emission directions provides unambiguous,

175

quantitative informations about the hole character and

176

the valence band mixing.

177

III. EXPERIMENTAL SETUP AND RESULTS

178

A. Sample fabrication

179

Figure 2. (a), µPL spectrum of ZnTe core and CdTe quantum dot luminescence, along with the integrated spectral range for cathodoluminescence imaging. (b), SEM image of the nanowire along with (c), spectrally resolved CL image and SEM image superimposed and (d), cut profile of the spec-trally resolved CL signal along the nanowire axis. The con-tribution of each part of the spectrum is coloured according to the spectrum in (a).

Our system is a single (Cd,Mn)Te QD inserted

180

along a <111> ZnTe/(Zn,Mg)Te core/shell nanowire

181

grown by molecular beam epitaxy (see Supplemental

182

Material28_{).}29,30_{The dot is largely doped with Mn atoms}

183

(Mn concentration ∼10%), making it a dilute magnetic

184

semiconductor structure. Due to the nature of the

185

growth, the axial core growth after the quantum dot

186

insertion leads to the formation of a ZnTe shell. A

fi-187

nal (Zn,Mg)Te shell is further grown on the resulting

188

tapered-shape nanowire. The wire is standing

perpen-189

dicular to the substrate in a region of low nanowire

190

density, allowing its study by micro-photoluminescence

191

(µPL) without exciting its neighbours. The PL spectrum

192

at 5K [Fig. 2(a)] exhibits an emission peak centered at

193

2.35 eV, which is related to the exciton recombination in

194

the ZnTe core,19,29,31 _{and a second one at 1.96 eV, which}

195

is attributed to the quantum dot luminescence. The

pres-196

ence of the Mn atoms significantly broadens the

emis-197

sion from the QD because of the magnetization

fluctua-198

tions randomly shifting the exciton line in time through

199

the giant Zeeman effect. The nanowire is also studied

200

by low-temperature cathodoluminescence (CL). The

elec-201

tron beam is along axis y. The standard SEM image [Fig.

202

2(b)] gives access to the geometrical parameters of the

203

wire. The CL signal [Fig. 2(c-d)] provides information

204

about the regions from where light is emitted. Most of

205

the ZnTe luminescence comes from a large region at the

206

base of the nanowire, while the signal attributed to the

207

quantum dot is well localized at a height of 1.8 µm from

208

the nanowire base. We note that the spatial width of

209

this signal is related to the diffusion of free electron and

210

holes in the nanowire before they recombine in the dot. It

211

does not correspond to the QD size (∼10 nm, measured

212

independently by energy-dispersive x-ray spectroscopy.32

213

CL spectroscopy on similar structures confirms that the

214

well-isolated emission line at 1.96 eV, which is also well

215

spatially confined, is related to a single longitudinal QD,

216

while eventual radial (Cd,Mn)Te structures would emit

217

at a higher energy, above 2.1 eV.33_{Finally, antibunching}

218

experiment on similar emitters without magnetic

dop-219

ing revealed a single photon emission with g2_{(0) = 0.35}_{,}

220

confirming the 3D confinement of the carriers inside the

221

dot.34 _{Such experiment could not be performed on our}

222

magnetically-doped dots yet because of the line

broaden-223

ing resulting from the large magnetic doping of the dot.

224

B. Fourier microscopy results

225

Let us first compare the unpolarised far field radiation

226

pattern of the ZnTe emission [Fig. 3(a)] to the one of the

227

QD [Fig. 3(c)]. Both present a single lobe of emission

228

whose center is slightly displaced from the origin. We

229

attribute this off-centering to a geometrical 5◦ _{tilt of the}

230

NW axis with respect to z, different from the previous

231

QD β tilt previously introduced in the spin Hamiltonian.

232

However, we note on the cross-sections that the

angu-233

lar divergence of the ZnTe emission is definitely smaller

234

than the QD one, which features a dip at its center.

235

This is a first hint for a LH emission from the QD as

236

the π transition reinforces light emission at large angles

237

[Fig. 1(d)]. Independent measurements of the objective

238

collection efficiency show that the latter drops

dramat-239

ically for sin θ ≥ 0.45 (see Supplemental Material (28_{).}

240

This does not affect the comparison between the two

241

lines, but prevent us to attempt a direct comparison with

242

the calculated patterns of Fig. 1(c-d). Another issue is

243

that the ZnTe emission takes place in a region where the

244

nanowire diameter is such that it strongly guides light

245

along the axis. Even more, due to the nanowire cone

246

shape, the guided mode waist increases adiabatically, and

247

hence its angular divergence decreases - a mechanism

248

which is exploited in photonic wires to maximize light

collection from single QD.5,24 _{On the contrary, at the}

250

QD location the nanowire diameter is too small to allow

251

an efficient guiding effect.

252

The difference between ZnTe and QD emission is

dra-253

matically highlighted when comparing their linearly

po-254

larised radiation patterns. In the case of ZnTe emission

255

they remains similar to the unpolarised one, whatever the

256

polariser direction. On the contrary, the QD emission

257

patterns break the revolution symmetry around z. We

258

observe two lobes, off-centered and symmetrically placed

259

on both sides of the optical axis along the direction of

260

polarisation. The lobe intensity decreases at large θ

an-261

gle because of the loss of collection efficiency otherwise

262

it would be maximum at the edge of the image as in

263

Fig. 1(b). We also note that there is a ∼20% intensity

264

imbalance between the two lobes. A convenient way to

265

reinforce the information about the polarisation state of

266

the far field, without the influence of its intensity, is to

267

plot the Stokes parameters35 _{S}

1 = (I0− I90)/(I0+ I90)

268

and S2= (I45−I135)/(I45+I135), where Iαis the far field

269

intensity for a linear polariser set at angle α. The degree

270

of linear polarisation (DLP) is equal to S2

1+ S22. In the

271

case of the ZnTe line, both Stokes parameters are

homo-272

geneous and very close to 0, with a DLP averaged over

273

all measured directions of light ∼2%. On the contrary,

274

the QD Stokes parameters are varying with ϕ from very

275

large positive values to very negative ones, displaying a

276

characteristic 4-quadrant symmetry. S2 is similar to S1

277

rotated by 45◦_{. The average DLP is ∼40%. This is a }

di-278

rect consequence of the polarisation properties sketched

279

in green in Fig. 1(c-d).

280

Experimental results were compared to far field

pat-281

terns derived from simulations of the electromagnetic

282

field in the whole nanowire structure by a finite element

283

software and taking into account all the experimental

284

imperfections of our imaging setup (see Supplemental

285

Material28_{). The emitter is modeled by an oscillating}

286

dipole d = dxx + dyy + dzz. The dipole matrix elements

287

diare determined by diagonalizing the hole Hamiltonian

288

including valence band mixing, and considering all

pos-289

sible transitions between the ground hole state and the

290

electron states. For the ZnTe core [Fig. 3(b)], we sum

291

the intensities coming from dipoles emitting at different

292

positions along the nanowire axis, with weights

corre-293

sponding to the CL intensity in Fig. 2(d). For the QD

294

[Fig. 3(d)], the dipole is fixed at the QD position. The

295

agreement with experimental data is very good.

Look-296

ing at the unpolarised QD pattern, the effects of the

va-297

lence band mixing rates σ/∆LH and ρ/∆LH are

entan-298

gled. However, the unbalanced intensity lobes (central

299

pannel) reflect σ/∆LH with its phase, while the linear

300

polarisation observed on S1 close to the optical axis

re-301

flects ρ/∆LH and its phase. The mixing rates are small,

302

hence the QD hole state is essentially (∼97%) LH. Yet

303

non zero valence band mixing is necessary to properly

304

explain the fine features found in the experimental data.

305

C. Magneto-optical spectroscopy

306

The analysis of the QD lines under magnetic field

(Zee-307

man splitting and circular polarisation degree) provides

308

another way to discriminate between LH and HH

exci-309

tons. In our experiment, the magnetic field is applied

310

along the NW axis (Faraday configuration). In non

mag-311

netic quantum dots with moderate exciton Landé factors,

312

large magnetic fields are usually required in order to lift

313

exciton spin manifold degeneracy. In (Cd,Mn)Te

mag-314

netic quantum dots, Mn atoms introduce localized spins

315

S = 5/2randomly distributed in the dot. The large

ex-316

change interaction between Mn spins and confined

carri-317

ers (electrons and holes) induces the so-called giant

Zee-318

man splitting of the exciton lines at low temperature

319

(effective Landé factor ∼100), which scales

proportion-320

ally to the normalized quantum dot magnetic moment

321

M/Msat(see section I in the Supplemental Material28).36

322

Even higher values are obtained with colloidal quantum

323

dots.37 _{In this case the strong anisotropy due to the}

324

wurtzite crystal structure enforces a heavy-hole

charac-325

ter. Fig. 4(a) shows the Zeeman energy diagram of

elec-326

trons and holes in an (Cd,Mn)Te/ZnTe QD with a 10%

327

Mn concentration under a magnetic field applied along

328

the z axis and assuming ∆LH < 0. At low

tempera-329

ture and for magnetic fields larger than a fraction of T,

330

photo-carriers relax to the lowest energy levels (|−1/2i

331

for electrons and |+1/2i for holes). This induces both

332

a red shift of the LH exciton line (black dashed arrow

333

in Fig. 4(a), and a strong linear polarisation along z (π

334

polarisation), according to the optical selection rules

re-335

called in Fig. 1(a). With the opposite assumption of a

336

HH ground state, we would expect a σ+ _{polarisation.}

337

In our experimental configuration, the magnetic field

338

is applied along the NW axis which still stands along

339

the optical axis (Faraday configuration), and the QD

lu-340

minescence is collected over an angular range of NA =

341

0.4. Figure 4(b) shows the quantum dot emission spectra

342

resolved in σ+ _{and σ}− _{polarisations for an applied }

mag-343

netic field of 0 T and 11 T. The emission at zero field

344

is dominated by the line at 1.962 eV previously studied

345

in far-field. At 11 T (corresponding to M/Msat ' 0.84

346

at T =10 K), the spectrum consists in two main lines at

347

1.94 eVand 1.953 eV. Both spectra present a weak

satel-348

lite line at higher energy whose origin is unclear. The

349

two lines are probably not related and a rather small

350

Zeeman shift is observed (see Fig. 5 in Appendix A). It

351

could be related to the luminescence from the substrate,

352

or from parasitic growth which takes place between the

353

nanowires. The Zeeman shift of the two main lines as a

354

function of the QD magnetic moment M/Msatis reported

355

in Fig. 4(c). The first line, observed for all magnetic

356

field values, presents a redshift proportional to M/Msat.

357

The shift at saturation is 25 meV as expected for a LH

358

exciton in a Cd0.9Mn0.1Te magnetic QD (see Appendix

359

A). It shows very moderate circular polarisation

imbal-360

ance, as expected for a LH emission which is ideally π

361

polarised. It confirms the LH exciton character of this

5

Figure 3. Coordinate system is the same as in Fig 1(c). In each panel we present the normalized unpolarised far field radiation diagram with two cross sections along the direction of the red and green arrows, the linearly polarised radiation diagrams at {0o

, 90o} and {45o

, 135o} sharing the same normalization factor (direction of polariser is indicated by gray arrow), and the S1 and S2 stokes parameter maps. (a), experimental results for the ZnTe emission line. (b), corresponding simulation results (ρ/∆LH = 0.14, σ/∆LH = 0.24, ψ = 112◦, χ = 186◦, or conversely ρ0/∆LH0= 0.14, ˆα = 100◦, ˆβ = 5◦ and ˆγ = 12◦). (c), experimental results for the QD emission line. (d), corresponding simulations (ρ/∆LH= −0.23, σ/∆LH = −0.06, ψ = 170◦, χ = 137◦, or conversely ρ0/∆LH0= −0.23, ˆα = 20◦, ˆβ = 16◦and ˆγ = 150◦).

line, as claimed by the analysis of farfield patterns in

363

zero magnetic field. The second line is clearly present

364

for fields larger than 6 T (M/Msat> 0.6). It is strongly

365

σ+ _{polarised. It also redshifts proportionally to M/M}
sat

366

with a shift at saturation of 37 meV. This value is

def-367

initely larger than the maximum possible LH Zeeman

368

shift, whatever the Mn content, of 25 meV. For these

369

two reasons, we ascribe this line to the |−1/2i → |3/2i

370

transition [red arrow in Fig. 4(a)] associated to the HH

371

exciton. The saturation shift is lower than the value

372

expected for a heavy-hole fully confined inside the dot

373

(51 meV), suggesting a rather weak confinement of the

374

HH excited state in the dot. At low field the behaviour

375

of the line is complicated due to coupling to LH states.

376

By extrapolating the Zeeman shift of the transition

ob-377

served at high field down to B =0 T we obtain a splitting

378

∆LH = −22 meV. We want to stress here that the

dif-379

ference in the polarization of the two lines is a strong

380

indication of the different nature of the hole involved in

381

each transition, and rules out the possible emission from

382

regions with different Mn content.

383

Information about the valence band mixing can be

re-384

trieved by a detailed analysis of the third Stokes

param-385

eter S3=

I_{σ+}−I_{σ−}

I_{σ+}+I_{σ−}, plotted in Fig. 4(d) S3. The strong

386

σ+ _{polarisation of the HH exciton line fully corresponds}

387

to the radiative recombination of a |−1/2i electron with

388

a |+3/2i hole, and the selection rules given in Fig. 1(a).

389

Surprisingly, one can note that the LH exciton line is

390

also partially circularly polarised at large magnetic field

391

(for M/Msat > 0.5). This partial circular polarisation

392

results from the hole mixing induced by the perturbation

393

term σe−iχ _{(see Supplemental Material}28_{). The black}

394

line in Fig. 4(d) give the theoretical variation of S3 for

395

the LH transition assuming a value of σ =3.9 meV

inde-396

pendent of the magnetic field and taking into account the

397

ratio in collection efficiency of π and σ polarised emission

398

fσπ = 1.8into the objective lens. The thermalization of

399

the holes between the Zeeman levels has been added in

400

order to get vanishing circular polarisation in zero field.

401

Using the hole energy levels deduced from the Zeeman

402

shifts of the exciton lines it yields σ ∆LH

2

'3%, in

agree-403

ment with the the simulations of the zero field emission

404

diagram. Due to the large value of fσπ, the mixing terms

405

do not affect S3 for the HH exciton at large magnetic

406

field: the red line in Fig. 4(d) displays the circular

polar-407

isation expected for the heavy hole exciton.

408

IV. DISCUSSION

409

The polarized emission diagram of the ZnTe nanowire

410

unambiguously reveals the HH character of the exciton,

411

with a small mixing. This is expected19_{from the presence}

412

of the (Zn,Mg)Te shell with a smaller lattice parameter;

413

the expected redshift was experimentally confirmed,29,38

414

and the heavy hole character was deduced from the

gi-415

ant Zeeman effect and the circular polarization observed

416

with a (Zn,Mn)Te core. Using the composition profile

417

obtained from Ref. 32 for a nanowire from the same

418

sample, and analytical expressions of the strain-induced

Figure 4. (a), Zeeman diagram of the electron and hole
confined levels split by the exchange interactions with Mn
atoms. The dashed arrows labeled XLH (resp. XHH)
corre-sponds to the LH (resp. HH) exciton transitions. The
low-energy transition involving a LH creates a |−1/2i electron in
the conduction band and a |+1/2i hole in the valence band,
hence it is linearly polarized along the z-axis. The low-energy
transition involving a HH creates a |−1/2i electron in the
con-duction band and a |+3/2i hole in the valence band, hence
it is σ+_{-polarized. (b), Photoluminescence spectra of the QD}
emission line recorded at 10K in zero field and at B=11T
(corresponding to a QD magnetic moment M/Msat= 0.84).
The magnetic field is applied along the nanowire axis oriented
parallel to the optical axis. Both circular polarisations (σ+_{in}
green and σ−_{in dashed blue) are shown. The intensity of the}
zero field spectrum has been multiplied by 2.5. (c), Zeeman
shift of the LH and HH exciton lines proportional to the QD
magnetic moment M/Msat. The continuous lines correspond
to the theoretical shift expected for a (Cd,Mn)Te quantum
dot with a Mn concentration of 10% (see text). (d), Circular
polarisation rates of the LH and HH exciton lines under
mag-netic field. The continuous lines corresponds to the expected
values taking into account the valence band mixing induced
by a constant perturbation term |σ| = 3.9 meV.

splitting,19,29 _{we expect ∆}

LH ' +30 meV and a ZnTe

420

emission energy around 2350 meV in agreement with

421

Fig. 2(a). This is consistent with the 50 meV value

de-422

duced from the anisotropy of the giant Zeeman effect

423

in (Zn,Mn,Te)/(Zn,Mg,Te) nanowires including a larger

424

Mg content.39 _{The mismatch between CdTe and ZnTe}

425

is opposite, so that we expect a LH character for a

426

hole confined in a core-shell nanowire19 _{or an elongated}

427

dot.18 _{For InAs/InP, a local splitting ∆}

LH '−100 meV

428

is calculated18_{at the center of a cylinder-shape QD with}

429

an aspect ratio 2, but due to an inhomogeneous strain

430

the HH state is ∼25 meV above the ground state. In

431

the present case, the aspect ratio is of the same order,

432

the mismatch slightly larger, but the CdTe-ZnTe valence

433

band offset is small so that another competition is

ex-434

pected with heavy-holes confined in the shell due to the

435

shear strain around the dot.19 _{A full calculation of ∆}
LH

436

is beyond the scope of this paper, but our measured value

437

is of the right order or magnitude.

438

We measure a value of the mixing term ρ0 ' 5meV.

439

Larger values have been reported for self-assembled

440

(Stranski-Krastanov) quantum dots.25 _{Actually, an }

im-441

portant feature is the symmetry of the principal axis, and

442

switching from the < 001 > to the < 111 > orientation

443

dramatically reduces in-plane asymmetry expected,40

444

and measured.41,42 _{Our dots are embedded in nanowires}

445

grown along the < 111 > axis. However the section of

446

such nanowires easily feature some ellipticity, of the

or-447

der of a few %, easily detected on the shell32 _{(although}

448

well beyond the resolution on the dot). A first evaluation

449

of the strain in an elongated (aspect ratio ∼ 2) ellipsoid

450

with some in-plane ellipticity can be done using the

Es-451

helby calculation:43,44 _{using the Bir-Pikus Hamiltonian,}

452

an ellipticity of 5% gives the right order of magnitude

453

for ρ0. Note that the same orientation of the ellipticity

454

will change the phase of ρ with the sign of the mismatch,

455

as observed between the dot and the ZnTe core. Finally,

456

writing the stiffness matrix with the < 111 > axis as

457

z-axis19 _{reveals that the presence of an in-plane shear}

458

(εxx− εyy) induces an axial shear stress, and hence a

459

strain εyz, of similar order of magnitude. This strain

460

gives rise to a non-zero σ, which is not a tilt, but can be

461

compensated by a tilt. Such a term is evidenced on the

462

emission diagram of the quantum dot, while it is partly

463

screened by guiding effect in the case of the ZnTe

emis-464

sion.

465

We have performed measurements on a set of ∼ 40

466

NWQDs from the same sample mechanically deposited

467

on a substrate. As they lie horizontally and close to a

468

reflecting substrate which significantly disturbs the

far-469

field radiation pattern, we could not perform the same

470

characterization as for the as-grown wire. Nevertheless

471

polarization studies reveal that the sample is actually

472

close to the threshold between light-hole and heavy-hole

473

ground state,18_{thus leading to a large dispersion in }

emis-474

sion properties. A majority of the QDs (∼ 70%) emit

475

light linearly polarized along the NW axis, which in our

476

system is a good indication of a LH ground state. The

re-477

maining 30% emit light polarized perpendicularly to the

478

NW axis, thus clearly indicating a HH character.

479

To conclude, complementary experiments on a single

480

nanowire unambiguously demonstrate a LH exciton

emis-481

sion. They allow to evaluate the splitting ∆LH as well

482

as the valence band mixing parameters. The results are

483

in agreement with the predictions of strain effects due

484

to the presence of a shell around the wire. We

demon-485

strate that valence band engineering through strain and

486

confinement is possible using bottom up approach and

487

semiconducting nanowire growth.

7

ACKNOWLEDGMENTS

489

We acknowledge the help of Institut Néel optical

490

engineering team (CL, Fabrice Donatini). This work

491

was supported by the French National Research Agency

492

under contracts ANR-11-BS10-013, ANR-15-CE24-0029

493

and ANR-10-LABX-51-01, and Institut Universitaire de

494

France.

495

Appendix A: Magneto-optical spectroscopy

496

Figure 5a displays photoluminescence spectra recorded

497

at different values of the magnetic field applied along the

498

nanowire axis. Only the extreme field values are plotted

499

in Fig. 4a of the main text. Most salient features are

500

the intense low energy line, which is present at zero field

501

and displays a continuous red shift when increasing the

502

intensity of the field. Fig. 5b, the position of this line is

503

plotted for different values of the applied magnetic field

504

and three values of the temperature (spectra of Fig. 5a,

505

and spectra at two other temperatures, not shown), as a

506

function of 5µBB/kB(T + TAF). The phenomenological

507

parameter TAF describes the antiferromagnetic

interac-508

tions in Cd0.9Mn0.1Te, see above. The coincidence of the

509

three sets of data confirms that the shift is due to the

gi-510

ant Zeeman effect, and follows a Brillouin function with

511

a shift at saturation equal to 25 meV (solid line). Note

512

that this line exhibits only a small circular polarization.

513

The second salient feature is the strongly σ+_{-polarized}

514

line, visible at high field only. A weaker line is observed

515

at high field, with a small Zeeman shift, which we did not

516

identify (the nanowire is still on the substrate and

para-517

sitic growth takes place between the nanowires). Finally,

518

the spectra at low fields appear as quite complex, but

519

this is expected by the proximity of several hole sublevels

520

at these field values (in particular, |+3/2i and |−1/2i

521

which are expected to (anti)-cross at these field values,

522

see Fig. 4b of the main text, and probably excited states

523

of the |+1/2i hole).

524

Appendix B: Theoretical background

525

1. Anisotropy of the holes

526

In a bulk semiconductor with the zinc-blende or

dia-527

mond structure, the hole quadruplet is degenerate

(rep-528

resentation Γ8of the cubic group). The presence of strain

529

or confinement lifts this degeneracy. If a principal axis

530

of symmetry exists, the hole Hamiltonian is usually

writ-531

ten, in the {|3/2i ; |1/2i ; |−1/2i ; |−3/2i} basis quantized

532

along this axis, as:

533 H = −1 2∆LH −σe

−iχ _{ρe}−2iψ _{0}

−σeiχ 1

2∆LH 0 ρe −2iψ

ρe2iψ 0 1_{2}∆LH σe−iχ

0 ρe2iψ σeiχ −1 2∆LH

(B1)

Figure 5. Magneto-optical spectroscopy.

(a) Photoluminescence spectra at T = 10 K with a magnetic field applied along the nanowire axis, from B = 0 to 11 T by steps of 1 T. The spectra at 0 and 11 T are displayed in Fig. 4a of main text. (b) Plot of the position of the low energy line as a function of 5µBB/kB(T + TAF)

If ∆LH is larger than ρ and σ, the two Kramers

534

doublet defined by this Hamiltonian are usually called

535

light-hole and heavy-hole (even if these terms are not

536

always justified), with ∆LH the light-hole to

heavy-537

hole energy splitting (the exact value of the splitting is

538

p∆2

LH+ 4ρ2+ 4σ2).

539

Two well known examples of this Hamiltonian are the

540

Luttinger-Kohn Hamiltonian which describes the hole

541

states in the vicinity of the valence band maximum, and

542

the Bir-Pikus Hamiltonian which describes the coupling

543

to a uniform strain.45

544

We want to stress here that this Hamiltonian H is

545

much more general: if the hole quadruplet is isolated,

546

Hcan be considered as a spin Hamiltonian, i.e., as an

547

effective Hamiltonian operating within the quadruplet.46

548

Some care must be taken when excited states have to be

549

considered.47

550

Moreover, this effective Hamiltonian can be built as a

551

linear combination of the successive powers of a

pseudo-552

spin, with real coefficients. In the case of a J = 3/2

553

quadruplet, powers of the J operators up to 3 are enough,

554

and in the absence of an applied magnetic field, only

555

even powers have to be considered in order to fulfill the

556

Kramers degeneracy. As a result, the most general spin

557

Hamiltonian which describes the quadruplet at the top

558

of the valence band can be written J.A.J, where the

559

vectorial operator J is the (pseudo)-moment and A is a

560

real 3 × 3 matrix. In addition, due to the commutation

561

rules of J, A is symmetric. Note that the contribution of

562

order zero to the spin Hamiltonian is redundant with the

563

trace of A; both represent a rigid shift of the quadruplet,

564

and a proper choice of the zero of energy allows us to

565

set the trace of H (hence that of A) to zero, as done in

Eq. B1.

567

Using the 4 × 4 matrices representing the second

pow-568 ers of J in the |3 2i, | 1 2i, | − 1 2i and | − 3 2i basis of the 569

Γ8 quadruplet, with the third axis z as the quantization

570

axis45_{, the matrix elements of H are}

571 T r(H) = 5 4(Axx+ Ayy+ Azz) = 0 1 2∆LH = 1 2Axx+ 1 2Ayy− Azz ρe−2iψ = √ 3 2 (Axx− Ayy− 2iAxy)

σe−iχ= −√3(Axz− iAyz) (B2)

Expressions of the matrix elements of Eq. B1 (hence

572

those of A) for the Luttinger-Kohn of Bir-Pikus

Hamil-573

tonian are generally expressed in the cubic basis.27 _{}

How-574

ever other axes can be chosen; for instance, in the case

575

of a nanowire oriented along the < 111 > axis, as in

576

the present study, it is useful to choose this axis as the z

577

quantization axis.19_{If H represents the coupling to a }

uni-578

form strain (the Bir-Pikus Hamiltonian) for an isotropic

579

system, ∆LH is proportional to the axial shear strain

580

(1_{2}εxx+ 1_{2}εyy − εzz), ρe−2iψ to the shear strain in the

581

xy plane,

√ 3

2 (εxx− εyy− 2iεxy), and σe

−iχ _{to the }

com-582

bination −√3(εxz − iεyz) of the shear strains in planes

583

containing z. However, it must be kept in mind that such

584

a spin Hamiltonian is general and can describe other

fea-585

tures governing the hole states, such as for instance the

586

inhomogeneous strain expected in a quantum dot, or the

587

effect of a confinement potential with a low symmetry.

588

Now, as the matrix A is real and symmetric, a mere

589

rotation makes it diagonal, with the three (real)

eigen-590

values on the diagonal. Using these eigenaxes (x0, y0,

591

z0), the spin Hamiltonian still writes J.A.J, and it still

592

develops as in Eq. B1, but Eq. B2 shows that now all

593

matrix elements are real (including ρ), and σ = 0:

594
H =
−1
2∆LH0 0 ρ0 0
0 1_{2}∆LH0 0 ρ0
ρ0 0 1_{2}∆LH0 0
0 ρ0 0 −1_{2}∆LH0
(B3)
with Az0z0 =
1
3∆LH0, Ax0x0 = −
1
6∆LH0+
1
√
3ρ0 and
595
Ay0y0 = −
1
6∆LH0−
1
√

3ρ0. If the z0axis is chosen so that

596

Az0z0 is the eigenvalue with the largest absolute value, 597

then ρ0< |∆LH0|/2

√

3; the two Kramers doublet will be

598

considered as light holes and heavy holes quantized along

599

z0, with some mixing due to ρ0.

600

To sum up, the most general spin Hamiltonian

describ-601

ing the hole states is given by Eq. B1, where diagonal

602

elements are real numbers but non-diagonal elements are

603

complex numbers. Diagonalizing the corresponding

ma-604

trix A determines a rotation (i.e., three Euler angles)

605

to a new set of axes where ∆LH0 but also ρ0 are real

606

numbers and σ=0, Eq. B3.

607

Figure 6. Light Hole exciton dipole radiation (a)
Princi-pal axes (x0, y0, z0)of the ellipsoid defined by Eq. B6 and
cal-culated for ψ = 40◦_{, χ = 110}◦_{, ρ/∆}

LH= 0.1, σ/∆LH = 0.3
and E0/∆LH = 2. They are obtained by 3 rotations with
the Euler angles ˆα = 40◦_{, ˆ}

β = 19◦and ˆγ = 0◦. (b) Orienta-tion of the 3 elementary orthogonal linear dipoles associated to the light hole exciton. They are oriented along the axes (x0, y0, z0). The π (resp. σ) polarized exciton transitions are associated to the dipole along z0(resp. x0and y0). The figure is calculated for the same Euler angles as above and for the hole anisotropy parameters = 0.214 (ρ0/∆LH0 = 0.0406). The lengthes of the colored lines are proportional to the dipole magnitudes dx0, dy0 and dz0 (see text).

As the principal axes of A are those where the

Hamil-608

tonian H is real with a vanishing σ, so that the hole states

609

are most simple to write, it is useful to write the effect

610

of a rotation on A and H. We apply to A or H the

ro-611

tation exp(−iˆγJz) exp

−i ˆβJy

exp(−i ˆαJz) defined by

612

three Euler angles (ˆα, ˆβ, ˆγ), see Fig. 6. It is particularly

613

interesting - and technically simpler - to consider small

614

values of ˆβ, so that we keep only the first order in ˆβ or

615

sin ˆβ. In this case, (ˆα + ˆγ) is the total angle of rotation

616

around the z axis (which has an effect only if the system

617

does not feature circular symmetry, with non vanishing

618

ρ0and different values of Ax0x0 and Ay0y0), while ˆβ is the 619

angle of the tilt and ˆγ its direction. The rotation matrix

620 in real space is 621 R =

cos( ˆα + ˆγ) − sin( ˆα + ˆγ) sin ˆβ cos ˆγ sin( ˆα + ˆγ) cos( ˆα + ˆγ) sin ˆβ sin ˆγ − sin ˆβ cos ˆα sin ˆβ sin ˆα 1

(B4)

and the matrix elements of A in the laboratory frame

622

are obtained by a straightforward calculation of RAt_{R}_{.}

623

H is derived using Eq. B2, or calculated directly using

624

the rotation exp(−iˆγJz) (1 − i ˆβJy) exp(−i ˆαJz), where

625

the operator of rotation around y (the tilt) is linearized.

626

The result is quite simple. The hamiltonian assumes the

627

form of Eq. B1, where:

9

1

2∆LH = 1 2∆LH0 ρe−2iψ = ρ0e−2i( ˆα+ˆγ)

σe−iχ= ˆβ( √

3

2 ∆LH0+ ρ0e

−2i ˆα_{)e}−iˆγ _{(B5)}

These expressions have been used to fit the

experimen-629

tal data.

630

2. Geometrical visualizing of the anisotropy tensor

631

Since in the case of the Bir-Pikus Hamiltonian, the

632

anisotropy matrix A is proportional to the strain tensor

633

(possibly weighted by the deformation potential

parame-634

ters), it is often quite illuminating to pursue the analogy

635

and to consider an ellipsoid defined in real space using

636

the matrix A, as an easy way to view the anisotropy

637

within the hole quadruplet. One possibility is to

con-638

sider a sphere of radius unity, to which we apply a strain

639

−Aij/E0, with an arbitrary scaling factor E0. If E0 is

640

larger than the largest eigenvalue of A, the result is an

641

ellipsoid which admits the x0, y0, z0 eigen-axes of A as

642

principal axes, with a half-axis length 1−Ax0x0/E0along 643

x0, and so on.

644

To first order in Aij/E0, the equation of such a solid

645 is 646 X i,j xi(δij+ 2Aij/E0)xj = 1 (B6)

where the xi’s are the coordinates x, y, z of an arbitrary

647

frame.

648

The principal axes of the ellipsoid are those where H

649

is real with σ = 0. A heavy-hole ground state implies

650

∆LH0> 0, and the ellipsoid is oblate (flat). A light-hole

651

ground state corresponds to a prolate (elongated)

ellip-652

soid. The in-plane ellipticity is measured by ρ0. An

ex-653

ample relevant for the present study is given in Fig. 6(a).

654

1 _{P. Michler, Science 290, 2282–2285 (2000).}

655

2 _{A. Zrenner, E. Beham, S. Stufler, F. Findeis, M. Bichler,}

656

and G. Abstreiter, Nature 418, 612–614 (2002).

657

3 _{A. J. Shields, Nature Photon 1, 215 (2007).}

658

4 _{C. Santori, M. Pelton, G. Solomon, Y. Dale, and Y. }

Ya-659

mamoto, Physical Review Letters 86, 1502–1505 (2001).

660

5 _{J. Claudon, J. Bleuse, N. S. Malik, M. Bazin, P. Jaffrennou,}

661

N. Gregersen, C. Sauvan, P. Lalanne, and J.-M. Gérard,

662

Nature Photonics 4, 174 (2010).

663

6 _{C. Santori, D. Fattal, J. Vučković, G. S. Solomon, and}

664

Y. Yamamoto, Nature 419, 594–597 (2002).

665

7 _{N. Akopian, N. H. Lindner, E. Poem, Y. Berlatzky,}

666

J. Avron, D. Gershoni, B. D. Gerardot, and P. M. Petroff,

667

Physical Review Letters 96, 130501 (2006).

668

8 _{A. Dousse, J. Suffczyński, A. Beveratos, O. Krebs,}

669

A. Lemaître, I. Sagnes, J. Bloch, P. Voisin, and P.

Senel-670

lart, Nature 466, 217–220 (2010).

671

9 _{D. V. Bulaev and D. Loss, Physical Review Letters 95,}

672

076805 (2005).

673

10 _{D. Heiss, S. Schaeck, H. Huebl, M. Bichler, G. Abstreiter,}

674

J. J. Finley, D. V. Bulaev, and D. Loss, Physical Review

675

B 76, 241306 (2007).

676

11 _{D. Sleiter and W. F. Brinkman, Physical Review B 74,}

677

153312 (2006).

678

12 _{D. E. Reiter, T. Kuhn, and V. M. Axt, Physical Review}

679

B 83, 155322 (2011).

680

13 _{H. Kosaka, T. Inagaki, Y. Rikitake, H. Imamura, Y. }

Mit-681

sumori, and K. Edamatsu, Nature 457, 702–705 (2009).

682

14 _{G. Bester, S. Nair, and A. Zunger, Physical Review B 67,}

683

161306 (2003).

684

15 _{L. He, G. Bester, and A. Zunger, Physical Review B 70,}

685

235316 (2004).

686

16 _{Y. H. Huo, B. J. Witek, S. Kumar, J. R. Cardenas,}

687

J. X. Zhang, N. Akopian, R. Singh, E. Zallo, R. Grifone,

688

D. Kriegner, and et al., Nat Phys 10, 46–51 (2013).

689

17 _{Y.-M. Niquet and D. C. Mojica, Physical Review B 77,}

690

115316 (2008).

691

18 _{M. Zieliński, Phys. Rev. B 88, 115424 (2013).}

692

19 _{D. Ferrand and J. Cibert, Eur. Phys. J. Appl. Phys. 67,}

693

30403 (2014).

694

20 _{A. Lafuente-Sampietro, H. Boukari, and L. Besombes,}

695

Physical Review B 92, 081305(R) (2015).

696

21 _{H. E. Ruda and A. Shik, Journal of Applied Physics 100,}

697

024314 (2006).

698

22 _{J. Bleuse, J. Claudon, M. Creasey, N. S. Malik, J.-M.}

699

Gérard, I. Maksymov, J.-P. Hugonin, and P. Lalanne,

700

Physical Review Letters 106, 103601 (2011).

701

23 _{G. Grzela,} _{R. Paniagua-Domínguez,} _{T. Barten,}

702

Y. Fontana, J. A. Sánchez-Gil, and J. Gómez

Ri-703

vas, Nano Lett. 12, 5481–5486 (2012).

704

24 _{G. Bulgarini, M. E. Reimer, M. Bouwes Bavinck, K. D.}

705

Jöns, D. Dalacu, P. J. Poole, E. P. A. M. Bakkers, and

706

V. Zwiller, Nano Lett. 14, 4102–4106 (2014).

707

25 _{C. Tonin, R. Hostein, V. Voliotis, R. Grousson,}

708

A. Lemaitre, and A. Martinez, Phys. Rev. B 85, 155303

709

(2012).

710

26 _{T. Dietl, A. Haury, and Y. Merle d’Aubigné, Physical}

711

Review B 55, R3347–R3350 (1997).

712

27 _{G. L. Bir and G. Pikus, Symmetry and Strain-Induced }

Ef-713

fects in Semiconductors, edited by N. Y. Wiley (Wiley,

714

New York, 1974).

715

28 _{“See supplemental material at [url will be inserted by }

pub-716

lisher] for details on the nanowires growth process and the

717

experimental setups and information on the numerical

pro-718

cedure and theoretical developments.”.

719

29 _{A. Artioli, A., P. Rueda-Fonseca, P., P. Stepanov,}

720

P., E. Bellet-Amalric, M. Den Hertog, C. Bougerol,

721

Y. Genuist, F. Donatini, R. André, R., G. Nogues, and

722

et al., Applied Physics Letters 103, 222106 (2013).

723

30 _{P. Rueda-Fonseca, E. Bellet-Amalric, R. Vigliaturo,}

M. den Hertog, Y. Genuist, R. André, R., E. Robin, A.

Ar-725

tioli, P. Stepanov, D. Ferrand, and et al., Nano Lett. 14,

726

1877–1883 (2014).

727

31 _{P. Wojnar, M. Zielinski, E. Janik, W. Zaleszczyk, T. }

Woj-728

ciechowski, R. Wojnar, M. Szymura, L. Klopotowski, L. T.

729

Baczewski, A. Pietruchik, and et al., Applied Physics

Let-730

ters 104, 163111 (2014).

731

32 _{P. Rueda-Fonseca, E. Robin, E. Bellet-Amalric, M. }

Lopez-732

Haro, M. Den Hertog, Y. Genuist, R. André, A. Artioli,

733

S. Tatarenko, D. Ferrand, and et al., Nano Lett. 16,

734

1637–1642 (2016).

735

33 _{P. Wojnar, J. Płachta, W. Zaleszczyk, S. Kret, A. M.}

736

Sanchez, R. Rudniewski, K. Raczkowska, M. Szymura,

737

G. Karczewski, L. T. Baczewski, and et al., Nanoscale

738

8, 5720–5727 (2016).

739

34 _{P. Stepanov, Magneto-Optical Spectroscopy of Magnetic}

740

Semiconductor Nanostructures, Ph.D. thesis, Université

741

Grenoble Alpes (2013).

742

35 _{W. H. McMaster, Rev. Mod. Phys. 33, 8–28 (1961).}

743

36 _{T. Clément, D. Ferrand, L. Besombes, H. Boukari, and}

744

H. Mariette, Physical Review B 81, 155328 (2010).

745

37 _{R. Beaulac, L. Schneider, P. I. Archer, G. Bacher, and}

746

D. R. Gamelin, Science 325, 973–976 (2009).

747

38 _{P. Wojnar, E. Janik, L. T. Baczewski, S. Kret,}

748

E. Dynowska, T. Wojciechowski, J. Suffczyński, J.

Papier-749

ska, P. Kossacki, G. Karczewski, J. Kossut, and T.

Woj-750

towicz, Nano Lett. 12, 3404 (2012).

751

39 _{M. Szymura, P. Wojnar, Ł. Kłopotowski, J. Suffczyński,}

752

M. Goryca, T. Smole’nski, P. Kossacki, W. Zaleszczyk,

753

T. Wojciechowski, G. Karczewski, and et al., Nano Lett.

754

15, 1972–1978 (2015).

755

40 _{R. Singh and G. Bester, Physical Review Letters 103,}

756

063601 (2009).

757

41 _{T. Kuroda, T. Mano, N. Ha, H. Nakajima, H. Kumano,}

758

B. Urbaszek, M. Jo, M. Abbarchi, Y. Sakuma, K. Sakoda,

759

and et al., Physical Review B 88, 041306 (2013).

760

42 _{G. Juska, V. Dimastrodonato, L. O. Mereni, A. Gocalinska,}

761

and E. Pelucchi, Nature Photon 7, 527–531 (2013).

762

43 _{J. D. Eshelby, Proceedings of the Royal Society A: }

Math-763

ematical, Physical and Engineering Sciences 241, 376–396

764

(1957).

765

44 _{J. D. Eshelby, Proceedings of the Royal Society A: }

Math-766

ematical, Physical and Engineering Sciences 252, 561–569

767

(1959).

768

45 _{G. Fishman, Semi-Conducteurs, les Bases de la Théorie}

769

k.p, edited by L. E. de l’Ecole Polytechnique (Les Editions

770

de l’Ecole Polytechnique, 2010).

771

46 _{A. Abragam and B. Bleaney, Electron Paramagnetic }

Reso-772

nance of Transition Ions, edited by C. P. Oxford

(Claren-773

don Press - Oxford, 1970).

774

47 _{J.-W. Luo, G. Bester, and A. Zunger, Physical Review B}

775

92, 165301 (2015).